New metal chalcogenides found in MnN-1(Gd2-xInx)SN+2 (N = 3, 4, 5): syntheses, structures, and magnetic properties.
Liang, I. C.; Weng, C. Y.; Huang, C.; Chang, C. K.; Sheu, H. S.; Lin, J. G.; Hsu, K. F.; Dalton transactions (Cambridge, England : 2003) 46 (2017) 1228–1236; doi:10.1039/c6dt04382h

data_7041491
_publ_section_title
;
 New metal chalcogenides found in MnN-1(Gd2-xInx)SN+2 (N = 3, 4, 5):
 syntheses, structures, and magnetic properties.
;
_journal_issue                   4
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              1228
_journal_page_last               1236
_journal_paper_doi               10.1039/c6dt04382h
_journal_volume                  46
_journal_year                    2017
_chemical_formula_moiety         GdInMn2S5
_chemical_formula_sum            'Gd0.25 In0.25 Mn0.5 S1.25'
_chemical_formula_weight         135.56
_space_group_crystal_system      orthorhombic
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2016-11-16 deposited with the CCDC.
2016-12-15 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   3.7892(3)
_cell_length_b                   12.4109(10)
_cell_length_c                   15.4894(13)
_cell_measurement_reflns_used    1259
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.06
_cell_measurement_theta_min      3.28
_cell_volume                     728.43(10)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0295
_diffrn_reflns_av_unetI/netI     0.0212
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            2778
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.196
_diffrn_reflns_theta_min         2.630
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    16.891
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.5648
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    5.000
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       piece
_exptl_crystal_F_000             976.8
_refine_diff_density_max         1.020
_refine_diff_density_min         -1.040
_refine_diff_density_rms         0.310
_refine_ls_extinction_coef       0.00156(10)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.135
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     34
_refine_ls_number_reflns         538
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.135
_refine_ls_R_factor_all          0.0196
_refine_ls_R_factor_gt           0.0166
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0150P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0342
_refine_ls_wR_factor_ref         0.0351
_reflns_Friedel_coverage         0.000
_reflns_number_gt                500
_reflns_number_total             538
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c6dt04382h2.cif
_cod_data_source_block           011
_cod_depositor_comments
'Adding full bibliography for 7041491--7041494.cif.'
_cod_original_formula_sum        'Gd0.25 In0.25 Mn0.50 S1.25'
_cod_database_code               7041491
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              30259